Output from "TOTOPOL", (version 1.92, 17 Jul 2017, Mike Treacy).

Report for the framework in file "public/tmp/tmp_194_6_101613959_9glNb8.cif"

There are 144 T-atoms per unit cell
There are 288 O-atoms per unit cell

Framework density = 21.73 T-atoms per nm^3
Material density = 2.168 grams per cm^3 (excluding extra-framework material)
-------------------------------------------------------------------
-------------------------- T-O Analysis ---------------------------
-------------------------------------------------------------------
[Si] Ideal SiO distance = 1.610 Angstrom
T1  -- O1  = 1.4892 Angstrom
T1  -- O3  = 1.6237 Angstrom
T1  -- O2  = 1.7462 Angstrom
T1  -- O4  = 1.7251 Angstrom
      mean = 1.6460 Angstrom
        t1 = 0.124329  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.102304  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T2  -- O3  = 1.6232 Angstrom
T2  -- O5  = 1.5746 Angstrom
T2  -- O6  = 1.6100 Angstrom
T2  -- O7  = 1.6449 Angstrom
      mean = 1.6132 Angstrom
        t1 = 0.025986  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.016510  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T3  -- O4  = 1.7455 Angstrom
T3  -- O8  = 1.7490 Angstrom
T3  -- O9  = 1.6393 Angstrom
T3  -- O10 = 1.6060 Angstrom
      mean = 1.6849 Angstrom
        t1 = 0.083425  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.043983  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T4  -- O7  = 1.6042 Angstrom
T4  -- O10 = 1.5713 Angstrom
T4  -- O11 = 1.5853 Angstrom
T4  -- O12 = 1.6601 Angstrom
      mean = 1.6052 Angstrom
        t1 = 0.032777  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.025466  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T5  -- O12 = 1.6256 Angstrom
T5  -- O13 = 1.6439 Angstrom
T5  -- O14 = 1.6194 Angstrom
T5  -- O15 = 1.5757 Angstrom
      mean = 1.6162 Angstrom
        t1 = 0.038920  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.024603  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T6  -- O15 = 1.5587 Angstrom
T6  -- O16 = 1.5915 Angstrom
T6  -- O17 = 1.6050 Angstrom
T6  -- O18 = 1.6102 Angstrom
      mean = 1.5913 Angstrom
        t1 = 0.022997  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.013055  (0.0 is a perfect tetrahedron)

        T-O SUMMARY
          Range  = 1.4892 A <--> 1.7490 A
          Mean   = 1.6261 A
          StdDev = 0.0619 A

       t1 Range  = 0.0230 <-- 0.0547 --> 0.1243
       t2 Range  = 0.0131 <-- 0.0377 --> 0.1023

-------------------------------------------------------------------
------------------------- O-T-O Analysis --------------------------
-------------------------------------------------------------------
O1  -- T1  -- O3  = 100.920 deg; O1  -- O3  = 2 A
O1  -- T1  -- O2  =  93.162 deg; O1  -- O2  = 2 A
O1  -- T1  -- O4  =  86.657 deg; O1  -- O4  = 2 A
O3  -- T1  -- O2  = 115.521 deg; O3  -- O2  = 3 A
O3  -- T1  -- O4  = 114.148 deg; O3  -- O4  = 3 A
O2  -- T1  -- O4  = 129.378 deg; O2  -- O4  = 3 A
       86.657 deg <-- 106.631 deg --> 129.378 deg

O3  -- T2  -- O5  = 107.830 deg; O3  -- O5  = 3 A
O3  -- T2  -- O6  = 108.536 deg; O3  -- O6  = 3 A
O3  -- T2  -- O7  = 115.322 deg; O3  -- O7  = 3 A
O5  -- T2  -- O6  = 107.740 deg; O5  -- O6  = 3 A
O5  -- T2  -- O7  = 106.297 deg; O5  -- O7  = 3 A
O6  -- T2  -- O7  = 110.812 deg; O6  -- O7  = 3 A
       106.297 deg <-- 109.423 deg --> 115.322 deg

O4  -- T3  -- O8  = 126.734 deg; O4  -- O8  = 3 A
O4  -- T3  -- O9  = 107.116 deg; O4  -- O9  = 3 A
O4  -- T3  -- O10 = 105.624 deg; O4  -- O10 = 3 A
O8  -- T3  -- O9  = 109.084 deg; O8  -- O9  = 3 A
O8  -- T3  -- O10 = 104.282 deg; O8  -- O10 = 3 A
O9  -- T3  -- O10 = 100.997 deg; O9  -- O10 = 3 A
       100.997 deg <-- 108.973 deg --> 126.734 deg

O7  -- T4  -- O10 = 105.589 deg; O7  -- O10 = 3 A
O7  -- T4  -- O11 = 106.639 deg; O7  -- O11 = 3 A
O7  -- T4  -- O12 = 115.469 deg; O7  -- O12 = 3 A
O10 -- T4  -- O11 = 107.823 deg; O10 -- O11 = 3 A
O10 -- T4  -- O12 = 113.703 deg; O10 -- O12 = 3 A
O11 -- T4  -- O12 = 107.195 deg; O11 -- O12 = 3 A
       105.589 deg <-- 109.403 deg --> 115.469 deg

O12 -- T5  -- O13 = 118.911 deg; O12 -- O13 = 3 A
O12 -- T5  -- O14 = 109.271 deg; O12 -- O14 = 3 A
O12 -- T5  -- O15 = 100.681 deg; O12 -- O15 = 2 A
O13 -- T5  -- O14 = 108.162 deg; O13 -- O14 = 3 A
O13 -- T5  -- O15 = 108.287 deg; O13 -- O15 = 3 A
O14 -- T5  -- O15 = 111.330 deg; O14 -- O15 = 3 A
       100.681 deg <-- 109.440 deg --> 118.911 deg

O15 -- T6  -- O16 = 104.424 deg; O15 -- O16 = 2 A
O15 -- T6  -- O17 = 109.557 deg; O15 -- O17 = 3 A
O15 -- T6  -- O18 = 111.810 deg; O15 -- O18 = 3 A
O16 -- T6  -- O17 = 111.779 deg; O16 -- O17 = 3 A
O16 -- T6  -- O18 = 109.601 deg; O16 -- O18 = 3 A
O17 -- T6  -- O18 = 109.602 deg; O17 -- O18 = 3 A
       104.424 deg <-- 109.462 deg --> 111.810 deg

        O-T-O SUMMARY
          Range  = 86.6574 deg <--> 129.3777 deg
          Mean   = 109.0901 deg
          StdDev = 7.7223 deg

        O--O SUMMARY
          Range  = 2.2122 A <--> 3.1381 A
          Mean   = 2.6466 A
          StdDev = 0.1781 A

-------------------------------------------------------------------
------------------------- T-T-T Analysis --------------------------
-------------------------------------------------------------------
-------------------------------------------------------------------
------------------------- T-O-T Analysis --------------------------
-------------------------------------------------------------------
T1  -- O1  -- T1  = 149.189 deg ; T1  -- T1   2.8714 A

T1  -- O2  -- T1  = 131.799 deg ; T1  -- T1   3.1880 A

T1  -- O3  -- T2  = 151.403 deg ; T1  -- T2   3.1463 A

T1  -- O4  -- T3  = 159.906 deg ; T1  -- T3   3.4173 A

T2  -- O5  -- T2  = 170.635 deg ; T2  -- T2   3.1387 A

T2  -- O6  -- T2  = 130.411 deg ; T2  -- T2   2.9231 A

T2  -- O7  -- T4  = 121.506 deg ; T2  -- T4   2.8349 A

T3  -- O8  -- T3  = 141.197 deg ; T3  -- T3   3.2992 A

T3  -- O9  -- T3  = 123.424 deg ; T3  -- T3   2.8871 A

T3  -- O10 -- T4  = 140.104 deg ; T3  -- T4   2.9867 A

T4  -- O11 -- T4  = 157.536 deg ; T4  -- T4   3.1097 A

T4  -- O12 -- T5  = 117.098 deg ; T4  -- T5   2.8030 A

T5  -- O13 -- T5  = 118.975 deg ; T5  -- T5   2.8325 A

T5  -- O14 -- T5  = 172.899 deg ; T5  -- T5   3.2326 A

T5  -- O15 -- T6  = 123.654 deg ; T5  -- T6   2.7631 A

T6  -- O16 -- T6  = 153.126 deg ; T6  -- T6   3.0958 A

T6  -- O17 -- T6  = 123.524 deg ; T6  -- T6   2.8279 A

T6  -- O18 -- T6  = 126.959 deg ; T6  -- T6   2.8814 A


        T-O-T SUMMARY
          Range  = 117.0980° <--> 172.8995 deg
          Mean   = 139.6303 deg
          StdDev = 17.5982 deg

        T--T SUMMARY
          Range  = 2.7631 A <--> 3.4173 A
          Mean   = 3.0133 A
          StdDev = 0.1889 A

-------------------------------------------------------------------
------------------------ *** WARNINGS *** -------------------------
-------------------------------------------------------------------

SOME OXYGEN ATOMS ARE TOO CLOSE TO EACH OTHER
O1  -- O4  = 2.2122 A
O1  -- O4  = 2.2122 A

T-T-T analysis was not conducted.

SOME T-ATOM DISTANCES ARE OUTSIDE THE NORMAL RANGE
T1  has 5 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T1  -- T1  = 2.8714 Angstrom
  T1  -- T1  = 3.1880 Angstrom
  T1  -- T1  = 3.3694 Angstrom
  T1  -- T2  = 3.1463 Angstrom
  T1  -- T3  = 3.4173 Angstrom
T3  has 5 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T3  -- T1  = 3.4173 Angstrom
  T3  -- T3  = 2.8871 Angstrom
  T3  -- T4  = 2.9867 Angstrom
  T3  -- T3  = 3.2992 Angstrom
  T3  -- T3  = 3.0493 Angstrom
T5  -- T6  = 2.7631 Angstrom
T6  -- T5  = 2.7631 Angstrom

-------------------------------------------------------------------
---------------------- Topological Analysis -----------------------
-------------------------------------------------------------------
T1 (Si): multiplicity = 24
Coordination Sequence =
    1 4 10 20 36 58 80 109 152 199 244 290 343 413 499 583 654
TD10 = 913
Circuit symbol = 4.5.4.6.5.7_{2}
Weight = 15
Vertex symbol  = 4.5.4.6.5.12_{2}
Weight = 29

T2 (Si): multiplicity = 24
Coordination Sequence =
    1 4 10 19 32 50 73 101 138 187 240 291 344 408 486 570 655
TD10 = 855
Circuit symbol = 4.4.5.6.6.7_{2}
Weight = 16
Vertex symbol  = 4.4.5.6.6.8
Weight = 20

T3 (Si): multiplicity = 24
Coordination Sequence =
    1 4 11 23 39 61 89 124 162 202 251 310 376 439 500 572 660
TD10 = 967
Circuit symbol = 4.6.5.6.7_{2}.8
Weight = 15
Vertex symbol  = 4.6.5.6.8.12
Weight = 27

T4 (Si): multiplicity = 24
Coordination Sequence =
    1 4 9 18 31 47 68 99 138 181 233 290 350 416 483 556 638
TD10 = 829
Circuit symbol = 4.5.4.6.4.6
Weight = 10
Vertex symbol  = 4.5.4.8.4.12
Weight = 24

T5 (Si): multiplicity = 24
Coordination Sequence =
    1 4 8 14 25 40 58 82 120 173 227 278 335 403 480 555 625
TD10 = 752
Circuit symbol = 4.4.4.6.4.6
Weight = 9
Vertex symbol  = 4.4.4.8.4.12
Weight = 23

T6 (Si): multiplicity = 24
Coordination Sequence =
    1 4 8 12 17 26 43 71 108 150 198 254 316 379 443 514 595
TD10 = 638
Circuit symbol = 4.4.4.6.4.6_{2}
Weight = 12
Vertex symbol  = 4.4.4.6.4.8
Weight = 17

<TD10> = 825.667
Average ring size = 5.2544
